#------------------------------------------------------------------------------
#$Date: 2017-10-13 12:16:50 +0200 (vie 13 de oct de 2017) $
#$Revision: 201980 $
#$URL: svn://www.crystallography.net/cod/cif/2/30/00/2300010.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2300010
loop_
_publ_author_name
'Bolotina, Nadezhda B.'
'Hardie, Michaele J.'
'Pinkerton, A. Alan'
_publ_section_title
;
 Energetic materials: variable-temperature crystal structures of two
 biguanidinium dinitramides
;
_journal_issue                   6
_journal_name_full               'Journal of Applied Crystallography'
_journal_page_first              1334
_journal_page_last               1341
_journal_paper_doi               10.1107/S0021889803016182
_journal_volume                  36
_journal_year                    2003
_chemical_formula_sum            'C2 H8 N8 O4'
_chemical_formula_weight         208.16
_chemical_name_common            'biguanidinium mono-dinitramide'
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXTL
_cell_angle_alpha                84.9180(10)
_cell_angle_beta                 81.686(2)
_cell_angle_gamma                80.928(2)
_cell_formula_units_Z            2
_cell_length_a                   4.3114(3)
_cell_length_b                   9.3227(5)
_cell_length_c                   10.5781(6)
_cell_measurement_reflns_used    2147
_cell_measurement_temperature    150.0(10)
_cell_measurement_theta_max      22.24
_cell_measurement_theta_min      5.77
_cell_volume                     414.50(4)
_computing_cell_refinement       'Siemens SAINT, 1996b'
_computing_data_collection       'Siemens SMART, 1996a'
_computing_data_reduction        'Siemens SAINT, 1996b'
_computing_molecular_graphics    SHELXTL
_computing_publication_material  'SHELXTL and the Toledo cifomatic'
_computing_structure_refinement  SHELXTL
_computing_structure_solution    'SHELXTL (Sheldrick, 1997)'
_diffrn_ambient_temperature      150.0(10)
_diffrn_measurement_device       Platform
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0535
_diffrn_reflns_av_sigmaI/netI    0.0669
_diffrn_reflns_limit_h_max       5
_diffrn_reflns_limit_h_min       -5
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_number            5627
_diffrn_reflns_theta_max         28.29
_diffrn_reflns_theta_min         1.95
_exptl_absorpt_coefficient_mu    0.152
_exptl_absorpt_correction_T_max  0.990327
_exptl_absorpt_correction_T_min  0.724471
_exptl_absorpt_correction_type   'Empirical :Multipole Expansion'
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    1.668
_exptl_crystal_density_method    '?                 '
_exptl_crystal_description       block
_exptl_crystal_F_000             216
_exptl_crystal_size_max          0.06mm
_exptl_crystal_size_mid          0.15mm
_exptl_crystal_size_min          0.23mm
_refine_diff_density_max         0.331
_refine_diff_density_min         -0.334
_refine_ls_extinction_coef       0.028(11)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXTL
_refine_ls_goodness_of_fit_all   1.056
_refine_ls_goodness_of_fit_obs   1.107
_refine_ls_matrix_type           full
_refine_ls_number_parameters     160
_refine_ls_number_reflns         2053
_refine_ls_number_restraints     8
_refine_ls_restrained_S_all      1.057
_refine_ls_restrained_S_obs      1.108
_refine_ls_R_factor_all          0.0972
_refine_ls_R_factor_obs          0.0560
_refine_ls_shift/esd_max         0.000
_refine_ls_shift/esd_mean        0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0764P)²+0.0292P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_all         0.1502
_refine_ls_wR_factor_obs         0.1266
_reflns_number_observed          1375
_reflns_number_total             2053
_reflns_observed_criterion       >2sigma(I)
_cod_data_source_file            do0021.cif
_cod_data_source_block           I150K
_cod_depositor_comments
;
The following automatic conversions were performed:
'_symmetry_cell_setting' value 'Triclinic' changed to 'triclinic'
according to '/home/saulius/struct/CIF-dictionaries/cif_core.dic'
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 

The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Triclinic' changed to 'triclinic'
according to /home/saulius/struct/CIF-dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_values 1715 2011-07-08 13:25:40Z adriana 

The following automatic conversions were performed:

'_refine_ls_weighting_scheme' value 'calc
w=1/[\s^2^(Fo^2^)+(0.0764P)^2^+0.0292P] where P=(Fo^2^+2Fc^2^)/3' was
changed to 'calc'. New tag '_refine_ls_weighting_details' was
created. The value of the new tag was set to
'w=1/[\s^2^(Fo^2^)+(0.0764P)^2^+0.0292P] where P=(Fo^2^+2Fc^2^)/3'.

Automatic conversion script
Id: cif_fix_values 3143 2015-03-26 13:38:13Z robertas 
;
_cod_original_sg_symbol_H-M      P-1
_cod_database_code               2300010
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_aniso_label
_atom_site_aniso_U_11
_atom_site_aniso_U_22
_atom_site_aniso_U_33
_atom_site_aniso_U_12
_atom_site_aniso_U_13
_atom_site_aniso_U_23
O4 0.0277(9) 0.0118(8) 0.0328(9) 0.0044(7) 0.0030(7) -0.0020(7)
N1 0.0209(10) 0.0142(9) 0.0214(10) 0.0021(8) 0.0021(8) 0.0010(7)
O3 0.0303(9) 0.0171(8) 0.0250(9) -0.0012(7) 0.0088(7) 0.0007(7)
N3 0.0226(10) 0.0140(9) 0.0188(9) -0.0001(8) 0.0003(8) -0.0041(7)
O1 0.0257(9) 0.0225(9) 0.0254(9) 0.0053(7) 0.0061(7) -0.0015(7)
O2 0.0407(11) 0.0191(9) 0.0335(10) 0.0108(8) 0.0091(8) 0.0107(8)
N2 0.0246(10) 0.0141(9) 0.0174(9) 0.0009(8) 0.0001(8) -0.0010(7)
N6 0.0360(12) 0.0115(9) 0.0217(10) -0.0004(8) 0.0044(9) 0.0013(8)
N8 0.0253(11) 0.0208(10) 0.0220(10) 0.0079(9) 0.0000(8) -0.0005(8)
N4 0.0252(10) 0.0126(9) 0.0207(10) 0.0023(8) 0.0035(8) 0.0005(7)
C1 0.0217(11) 0.0132(10) 0.0191(11) 0.0024(9) -0.0002(9) -0.0003(8)
C2 0.0209(11) 0.0123(10) 0.0207(11) -0.0013(9) -0.0015(9) -0.0011(8)
N7 0.0255(11) 0.0199(10) 0.0198(10) 0.0042(9) 0.0020(8) -0.0014(8)
N5 0.0439(13) 0.0136(10) 0.0225(10) 0.0021(9) 0.0084(9) -0.0020(8)
loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_thermal_displace_type
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_occupancy
_atom_site_disorder_group
_atom_site_type_symbol
O4 -1.5634(4) 0.7804(2) 0.7452(2) 0.0255(4) Uani d . 1 . O
N1 -1.1565(4) 0.5873(2) 0.7080(2) 0.0199(4) Uani d . 1 . N
O3 -1.5470(4) 0.5756(2) 0.8595(2) 0.0258(4) Uani d . 1 . O
N3 -1.4325(5) 0.6555(2) 0.7697(2) 0.0188(4) Uani d . 1 . N
O1 -0.7664(4) 0.5948(2) 0.5555(2) 0.0265(4) Uani d . 1 . O
O2 -1.1280(5) 0.7838(2) 0.5577(2) 0.0349(5) Uani d . 1 . O
N2 -1.0192(5) 0.6633(2) 0.6025(2) 0.0194(4) Uani d . 1 . N
N6 -0.5251(5) 1.3145(2) 0.7025(2) 0.0244(5) Uani d D 1 . N
N8 -1.0245(5) 1.3123(2) 0.9109(2) 0.0243(5) Uani d D 1 . N
N4 -0.6112(5) 1.1173(2) 0.8554(2) 0.0208(5) Uani d . 1 . N
C1 -0.5107(5) 1.1727(2) 0.7386(2) 0.0188(5) Uani d . 1 . C
C2 -0.8266(5) 1.1918(2) 0.9398(2) 0.0182(5) Uani d . 1 . C
N7 -0.8503(5) 1.1382(2) 1.0605(2) 0.0231(5) Uani d D 1 . N
N5 -0.3751(6) 1.0782(2) 0.6521(2) 0.0286(5) Uani d D 1 . N
H7B -1.043(5) 1.169(3) 1.122(3) 0.050(9) Uiso d D 1 . H
H6A -0.568(8) 1.392(3) 0.766(2) 0.055(10) Uiso d D 1 . H
H7A -0.694(5) 1.055(2) 1.086(2) 0.025(7) Uiso d D 1 . H
H5A -0.248(6) 1.114(3) 0.5725(18) 0.038(8) Uiso d D 1 . H
H8B -1.186(6) 1.354(3) 0.981(2) 0.047(9) Uiso d D 1 . H
H8A -1.035(7) 1.353(3) 0.8210(14) 0.045(9) Uiso d D 1 . H
H5B -0.382(8) 0.9718(13) 0.671(3) 0.053(9) Uiso d D 1 . H
H6B -0.445(7) 1.342(3) 0.6116(13) 0.037(8) Uiso d D 1 . H
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
N3 N1 N2 116.2(2)
O4 N3 O3 121.4(2)
O4 N3 N1 127.0(2)
O3 N3 N1 111.5(2)
O2 N2 O1 122.6(2)
O2 N2 N1 125.9(2)
O1 N2 N1 111.5(2)
C1 N4 C2 123.4(2)
N5 C1 N4 117.0(2)
N5 C1 N6 117.4(2)
N4 C1 N6 125.5(2)
N7 C2 N8 117.8(2)
N7 C2 N4 116.8(2)
N8 C2 N4 125.4(2)
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
O4 N3 . 1.234(2) ?
N1 N3 . 1.363(2) ?
N1 N2 . 1.378(2) ?
O3 N3 . 1.247(2) ?
O1 N2 . 1.234(2) ?
O2 N2 . 1.228(2) ?
N6 C1 . 1.338(3) ?
N8 C2 . 1.340(3) ?
N4 C1 . 1.336(3) ?
N4 C2 . 1.345(3) ?
C1 N5 . 1.334(3) ?
C2 N7 . 1.325(3) ?
loop_
_cod_related_entry_id
_cod_related_entry_database
_cod_related_entry_code
1 ChemSpider 23078682
